세계 제일의 방대한 재료 데이터베이스

# Engineering Stress-strain Curve: Part Three

요약:

The engineering tension test is widely used to provide basic design information on the strength of materials and as an acceptance test for the specification of materials. In the tension test a specimen is subjected to a continually increasing uniaxial tensile force while simultaneous observations are made of the elongation of the specimen. The parameters, which are used to describe the stress-strain curve of a metal, are the tensile strength, yield strength or yield point, percent elongation, and reduction of area. The first two are strength parameters; the last two indicate ductility.

### Measures of Yielding

The stress at which plastic deformation or yielding is observed to begin depends on the sensitivity of the strain measurements. With most materials there is a gradual transition from elastic to plastic behavior, and the point at which plastic deformation begins is hard to define with precision. Various criteria for the initiation of yielding are used depending on the sensitivity of the strain measurements and the intended use of the data.
1. True elastic limit based on micro strain measurements at strains on order of 2 x 10-6 in | in. This elastic limit is a very low value and is related to the motion of a few hundred dislocations.
2. Proportional limit is the highest stress at which stress is directly proportional to strain. It is obtained by observing the deviation from the straight-line portion of the stress-strain curve.
3. Elastic limit is the greatest stress the material can withstand without any measurable permanent strain remaining on the complete release of load. With increasing sensitivity of strain measurement, the value of the elastic limit is decreased until at the limit it equals the true elastic limit determined from micro strain measurements. With the sensitivity of strain usually employed in engineering studies (10-4in | in), the elastic limit is greater than the proportional limit. Determination of the elastic limit requires a tedious incremental loading-unloading test procedure.
4. The yield strength is the stress required to produce a small-specified amount of plastic deformation. The usual definition of this property is the offset yield strength determined by the stress corresponding to the intersection of the stress-strain curve and a line parallel to the elastic part of the curve offset by a specified strain. In the United States the offset is usually specified as a strain of 0.2 or 0.1 percent (e = 0.002 or 0.001).
 (4)
A good way of looking at offset yield strength is that after a specimen has been loaded to its 0.2 percent offset yield strength and then unloaded it will be 0.2 percent longer than before the test. The offset yield strength is often referred to in Great Britain as the proof stress, where offset values are either 0.1 or 0.5 percent. The yield strength obtained by an offset method is commonly used for design and specification purposes because it avoids the practical difficulties of measuring the elastic limit or proportional limit.

Some materials have essentially no linear portion to their stress-strain curve, for example, soft copper or gray cast iron. For these materials the offset method cannot be used and the usual practice is to define the yield strength as the stress to produce some total strain, for example, e = 0.005.

### Measures of Ductility

At our present degree of understanding, ductility is a qualitative, subjective property of a material. In general, measurements of ductility are of interest in three ways:
1. To indicate the extent to which a metal can be deformed without fracture in metalworking operations such as rolling and extrusion.
2. To indicate to the designer, in a general way, the ability of the metal to flow plastically before fracture. A high ductility indicates that the material is "forgiving" and likely to deform locally without fracture should the designer err in the stress calculation or the prediction of severe loads.
3. To serve as an indicator of changes in impurity level or processing conditions. Ductility measurements may be specified to assess material quality even though no direct relationship exists between the ductility measurement and performance in service.
The conventional measures of ductility that are obtained from the tension test are the engineering strain at fracture ef (usually called the elongation) and the reduction of area at fracture q. Both of these properties are obtained after fracture by putting the specimen back together and taking measurements of Lf and Af .
 (5) (6)
Because an appreciable fraction of the plastic deformation will be concentrated in the necked region of the tension specimen, the value of ef will depend on the gage length L0 over which the measurement was taken. The smaller the gage length the greater will be the contribution to the overall elongation from the necked region and the higher will be the value of ef. Therefore, when reporting values of percentage elongation, the gage length L0 always should be given.

The reduction of area does not suffer from this difficulty. Reduction of area values can be converted into an equivalent zero-gage-length elongation e0. From the constancy of volume relationship for plastic deformation A*L = A0*L0, we obtain
 (7)
This represents the elongation based on a very short gage length near the fracture.

Another way to avoid the complication from necking is to base the percentage elongation on the uniform strain out to the point at which necking begins. The uniform elongation eu correlates well with stretch-forming operations. Since the engineering stress-strain curve often is quite flat in the vicinity of necking, it may be difficult to establish the strain at maximum load without ambiguity. In this case the method suggested by Nelson and Winlock is useful.

References

1. C. Moosbrugger: Representation of Stress-Strain Behavior, Atlas of Stress-strain Curves, ASM International, 2002, ISBN 087170739X and 9780871707390;

2. R. Gürbüz: Tension test, Experiment 1, Accessed May 2020.

## 기술 자료 검색

검색할 어구를 입력하십시오:

 검색 범위 본문 키워드 머릿글 요약

 이 문서는 전체 문서 중 일부분입니다. 이 주제에 대해 더 읽고 싶으시면 아래 링크를 클릭하시면 됩니다.

Total Materia Extended Range는 수천개 재질의 탄성 영역 범위 내 계산용 응력-변형률 곡선, 열처리 및 공정 온도 정보를 포함하고 있습니다. 다양한 변형률 속도에 따른 진응력-진변형률 곡선 및 공칭응력-공칭변형률 곡선 또한 제공됩니다.

응력-변형률 곡선을 데이터베이스에서 검색하는 것은 매우 쉽습니다.

신속 검색에 검색할 재질명을 입력합니다. 원하신다면 국가/규격을 지정하신 후 검색 버튼을 클릭합니다.

관심 소재를 선택한 후, 선택된 소재에 대한 응력-변형률 곡선의 링크를 클릭하십시오. 가능한 응력 - 변형률 곡선 기록의 개수는 링크 옆 괄호 안에 표시됩니다.

Total Materia 응력-변형률 곡선은 규격 사양서와 무관하므로, 어떠한 소그룹 내의 링크를 클릭하셔도 응력-변형률 곡선을 검토하실 수 있습니다.

온도가 달라지면 응력-변형률 곡선도 변하기 때문에, 응력과 변형률 정보는 표로 주어져 있습니다. 이는 CAE 소프트웨어 등에 쉽게 응용하실 수 있습니다.

다른 작동 온도에서 응력-변형률 곡선을 검토하실 수도 있습니다.

이를 위해서는 간단히 범위 내 새로운 온도를 온도 입력 창에 입력하시면 됩니다.

계산 버튼을 누르시면 새로운 온도와 그에 대응하는 값이 출력됩니다. 250°C에서의 예를 보십시오.

Total Materia 데이터베이스를 사용해 보실 수 있는 기회가 있습니다. 저희는 Total Materia 무료 체험을 통해 150,000명 이상의 사용자가 이용하고 있는 커뮤니티로 귀하를 초대합니다.